Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our User Agreement and Privacy Policy.

Slideshare uses cookies to improve functionality and performance, and to provide you with relevant advertising. If you continue browsing the site, you agree to the use of cookies on this website. See our Privacy Policy and User Agreement for details.

Like this document? Why not share!

805 views

Published on

http://www.ijmer.com/papers/Vol3_Issue3/AD3312791282.pdf

No Downloads

Total views

805

On SlideShare

0

From Embeds

0

Number of Embeds

4

Shares

0

Downloads

0

Comments

0

Likes

1

No embeds

No notes for slide

- 1. International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol.3, Issue.3, May-June. 2013 pp-1279-1282 ISSN: 2249-6645www.ijmer.com 1279 | PageParveen,1Ankit Sharma212Department of Civil Engineering DCRUST, Sonepat, Haryana, IndiaAbstract: The aim of the present study is to investigate the effect of variation of polypropylene fibres ranging from 0.1% to0.4% along with 0.8% steel fibres on the behaviour of fibrous concrete. The mechanical properties of the concrete such ascompressive and tensile strength have been investigated. The result shows that addition of polypropylene fibre has a littleeffect on the compressive strength, but there was significant increase in the tensile strength with increase in fibre volumefraction. The present investigation shows an increase of 47% of split tensile strength and 50% of flexural strength. The resultshows that ultimate load mainly depended on percentage volume fraction of fibre.Keywords: Ppf, Gfrp, Sfrc, Fbc, PfrcI. INTRODUCTIONConcrete is known to be a brittle material when subjected to tensile stresses and impact loads; tensile strength of theconcrete is approximately one tenth of its compressive strength. As a result of this, concrete members are unable to withstandsuch loads and stress that are usually encountered by concrete structural members. Usually, concrete members are reinforcedwith continuous reinforcing bars to withstand tensile stresses and to compensate for the lack of ductility and strength. Theaddition of steel reinforcement to concrete significantly increases its strength, but to produce a concrete with homogenoustensile properties and better micro cracking behaviour, fibres are advantageous. The introduction of fibres in concrete hasbrought a solution to develop a concrete having enhanced flexural and tensile strength, which are a new form of compositematerial. At the micro-level, fibres inhibit the initiation and growth of cracks, and after the micro-cracks coalesce intomacro-cracks, fibres provide mechanisms that abate their unstable propagation, provide effective bridging, and impartsources of strength gain, toughness and ductility. Fibres are mostly discontinuous, randomly distributed throughout thecement matrices.The randomly distributed short fibres are generally introduced into concrete to enhance its control crack system andmechanical properties such as toughness, impact resistance, ductility (post cracking), tensile strength etc. of basic matrix.There are many kinds of fibres, such as metallic, synthetic, natural etc which are being used in normal concrete as shown inFig 1. The term fibre based concrete (FBC) is concrete containing fibrous material which increases its structural integrity. Itcontains short discrete fibres that are uniformly distributed and randomly oriented. Different type of fibres in concretechanges the character of fibre based concrete. Further properties of fibre based concrete changes with varying concrete, fibrematerials geometries, distribution, orientation and densities. When fibre is added to a concrete mix, each and everyindividual fibre receives a coating of cement paste. Modification of synthetic fibre geometry includes monofilaments,fibrillated fibres, fibre mesh, wave cut fibre large end fibres etc. This increases bonding with cement matrices withoutincreasing in its length and minimized chemical interaction between fibres and the cement matrices. Fibres also modifies andenhances the mechanical properties and behaviour of concrete during its application. Fibre can be used with admixture suchas super plasticizer, air entraining, retarding, accelerating etc and all type of cement and concrete mixtures. These produce aspecial type of concrete with desired properties in fresh and hardened concrete. In present study polypropylene and steelfibres have been used. Polypropylene fibre having low modulus, light density, small monofilament diameter and notsusceptible to corrosion and steel fibre increases its ductility, toughness, and impact resistance. Polypropylene and steel fibreis(a) (b) (c)Figure 1. (a) polypropylene fiber (b) glass fiber (c) steel fiberConsidered to be an effective method for improving the shrinkage, cracking characteristics, toughness and impactresistance of concrete material Almost all FRCs used today commercially involve the use of a single fibre type. Clearly, aStructural Behaviour of Fibrous Concrete Using PolypropyleneFibres
- 2. International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol.3, Issue.3, May-June. 2013 pp-599-603 ISSN: 2249-6645www.ijmer.com 1280 | Pagegiven type of fibre can only be effective in a limited range of crack opening and deflection. The benefits of combiningorganic (polypropylene and nylon) and inorganic fibres (glass, asbestos and carbon) to achieve superior tensile strength andfracture toughness were recognized about 30 years back. Thereafter much research was not undertaken, recently again thereis renewed interest in this field. In present study the structural behaviour of the fibre based concrete using hybrid fibres hasbeen conducted.II. EXPERIMENT AND RESULTTo achieve the objectives of research programme, an experimental investigation has been carried out on FBC. Thecubes, cylinders & beams have been cast with varying percentages of fibre volume fraction. This chapter outlines theexperimental program plan, properties of the constituent materials, concrete mix, casting of specimen and testing of specimen.The focus of experimental investigation is to assess the structural behaviour of fibre based concrete. To attain the aim ofpresent study experimental investigation is carried out on 60 Nos. of fibre based reinforced concrete cubes, 60 nos. of fibrebased reinforced concrete cylinder & 60 Nos. of fibre based reinforced concrete beams, having overall dimensions (L x B x D)as 150 x 150 x 150 mm for cubes, for cylinder (L x D) as (300 x 150 mm) & for beams (L x B x D) as 500 x 100 x 100 mm.(a) (b) (c)Figure 2. (a) Setup for compressive strength (b) Setup for Split Tensile strength (c) Setup for Flexural strengthA. Compressive Strength –From the results it observed that the addition of the polypropylene fibre in the control mix has a little effect on thecompressive strength. It is observed that the use of fibres increases the compressive strength of concrete when thepolypropylene fibres were up to 0.2% and then reduction in compressive strength is observed. An increase in 7.5% incompressive strength occurs when the percentage of polypropylene fibre increases up to 0.2%. The decrease in compressivestrength is observed when percentage of fibres increases beyond 0.2%. The increase in the compressive strength is due to theincrease in bonding effect of fibre with matrix. With the increase in percentage volume of fibre beyond its optimum value(which is 0.2% in present case) compressive strength decreases, this is due to the increase in interference of fibre with eachother. This will produce internal voids in concrete mix which leads to decrease the total density of mix and thereby decreasethe compressive strength of the mix.Table -1 Compressive StrengthSr.No.Percentage of polypropylenefibre along with 0.8% steelfibreCompressivestrength(N/mm2)After 7 DaysCompressivestrength(N/mm2)After 28 Days1 0% 27.86 39.842 0%+0.8% 28.40 40.503 0.1%+0.8% 28.54 40.904 0.2%+0.8% 29.92 42.825 0.3%+0.8% 27.90 40.026 0.4%+0.8% 27.08 39.58B. Flexural Strength–It is observed that with the increase in polypropylene fibre, the flexural strength increases. However, it is noticed thatthe rate of increase of flexural strength is more as compared to compressive strength. The results show that optimum dosagefor flexure is 0.3% of polypropylene fibre along with 0.8% of steel fibre. The above results show that flexural strengthincreases with increase in fibre volume fraction; this is due to the additional load taken by the fibres present in the matrix.However, after increasing the volume percentage of polypropylene fibre beyond the optimum value (0.3%) improper mixingof fibres with the matrix takes place due to balling effect of fibre, this increases the amount of vibrations required to removeair voids from the mix which in turn causes the problem of bleeding and decreases flexural strength of the mix. The failurepattern of plain and hybrid fibrous concrete in flexural strength test shows that fibrous concrete are more ductile as comparedto plain concrete. This is because when the matrix cracked, the load was transferred from the composite to the fibres at thecrack surfaces, which prevents the brittle failure of the composite.
- 3. International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol.3, Issue.3, May-June. 2013 pp-599-603 ISSN: 2249-6645www.ijmer.com 1281 | PageTable -2 Flexural StrengthSr.No.Percentage of polypropylenefibre along with 0.8% steelfibreFlexural strength(N/mm2)After 7 DaysFlexural strength(N/mm2)After 28 Days1 0% 3.63 4.672 0%+0.8% 3.73 4.803 0.1%+0.8% 3.92 5.574 0.2%+0.8% 4.40 6.195 0.3%+0.8% 5.01 7.206 0.4%+0.8% 4.15 5.92C. Split Tensile Strength–For studying the split tensile behaviour, cylinders of fibrous concrete were tested. The failure load was observed andthe strength was calculated which is shown in Table 3. The figures show the effects of volume variation of polypropylene fibreand split tensile strength of concrete. It is noted that with the increase in the polypropylene fibres upto 0.3% the split tensionstrength increases. The above results shows that split tensile strength increases with increase in fibre volume fraction, becauseof the holding capacity of the fibres which helps in preventing the splitting of concrete. However, after increasing the volumepercentage of polypropylene fibre beyond the optimum value (0.3%) improper mixing of fibres with the matrix takes placedue to balling effect of fibre, this increases the amount of vibrations required to remove air voids from the mix which in turncauses the problem of bleeding and decreases split tensile strength of the mix.Table -3 Split Tensile StrengthSr.No.Percentage of polypropylenefibre along with 0.8% steelfibreSplit tensile strength(N/mm2)After 7 DaysSplit tensile strength(N/mm2)After 28 Days1 0% 2.14 3.102 0%+0.8% 2.25 3.353 0.1%+0.8% 2.59 3.724 0.2%+0.8% 2.83 4.095 0.3%+0.8% 3.50 4.956 0.4%+0.8% 2.70 3.85D. Stress Strain Response–Figure 3. Stress strain response of FBC at different volume fraction of polypropylene fibreAbove figure shows there is significant change in strain of the concrete due to addition of fibres. Descending portionof the curve becomes more and more flatten as the fibre volume fraction increases. The relationship with different volumefraction of polypropylene fibre is shown in Fig. 3. Two different behaviour patterns are obtained as shown in stress straincurve. The stress-strain behaviour of the specimens containing polypropylene fibre upto 0.1% behaves in a similar trend to thecontrol specimen. For these cases which contains 0% and 0.1% polypropylene fibre behaves like a brittle material of which thetotal energy is generated is elastic energy. However, non linear behaviour is seen for the other specimens which contains morethan 0.1% of polypropylene fibre. Here, once the peak stress is reached the specimens continues to yield as shown in figure 3.Therefore it can be stated that concrete with higher percentage of polypropylene fibre possess higher toughness, since thegenerated energy is mainly plastic. Also it was found that as fibre volume increase failure strain also increases, which leads tomore area under the curve, thus enhancing the toughness of the concrete.III. CONCLUSIONBased on experimental investigation and analysis of results obtained, the following conclusions may be drawn broadly:1. Steel-polypropylene mix shows a slight increase in the compressive strength as compared with the plain concrete. Hybrid(steel + polypropylene) fibre showed about 5.7% increase in compressive strength.2. It is observed that polypropylene fibre have not contributed significantly towards compressive strength.3. The maximum gain in compressive strength was achieved for 0.2% polypropylene fibre. Thereafter increase in fibrecontent has marginally reduced the compressive strength.4. Hybrid FRC (steel + polypropylene) shows an increase in split tensile strength as compared to the plain concrete. Fibrereinforced concrete mix showed a considerable increase of about 47% in split tensile strength.
- 4. International Journal of Modern Engineering Research (IJMER)www.ijmer.com Vol.3, Issue.3, May-June. 2013 pp-599-603 ISSN: 2249-6645www.ijmer.com 1282 | Page5. The maximum gain in split tensile strength was achieved for 0.3% polypropylene fibre. Thereafter increase in fibrecontent has marginally reduced the split tensile strength.6. Steel-polypropylene fibre reinforced concrete showed increase in flexural strength when compared with steel fibrereinforced concrete.7. The maximum gain in flexural strength was achieved for 0.3% polypropylene fibre. Thereafter increase in fibre contenthas marginally reduced the flexural strength.8. From the present study it is observed that the optimum dosage of polypropylene fibre fraction is 0.3%.9. Stress-Strain relationship showed that there was marginal increase in strain. Stress-Strain relationship shows that strainincreases as the percentage of polypropylene fibre increases. As fibre volume increases failure strain also increases, whichleads to more area under the curve, thus enhancing the toughness of concrete.Reference[1] A. Sivakumar, Manu Santhanam, “Mechanical properties of high strength concrete reinforced with metallic and non-metallic fibre”,cement and concrete composite 29 (2007) 603-608.[2] ASTM A820, “Steel fibre-reinforced concrete design consideration”, (1997).[3] Balaguru, P., and Ramakrishnan, V., Properties of Fiber Reinforced Concrete: Workability Behavior under Long Term Loading andAir-Void Characteristics", ACI Materials Journal, May-Jun, Vol. 85, No. 3, pp. 189-196,1988.[4] Chote Soranakom, Bazin Mobasher, “flexure design of fibre reinforced concrete”, ACI Material Journal (September 2009).[5] C.D. Johnston, “Steel fibre reinforced mortar and concrete”, A review of mechanical properties in fibre reinforced concrete ACI- SP44- Detroit (1974).[6] F.Puertas, T.Amat, Fernandez-Jimenez, T.Vazquez, “Mechanical and durable behavior of alkaline cement mortars reinforced withpolypropylene fibres”, Cement and Concrete Research 33 (2003) 2031-2036.[7] Giuseppe Campione, Maria Letizia Mangiavillano, “fibrous reinforced concrete beam in flexure: experimental investigation,analytical modeling and design considerations” Engineering structures journal 30 (2008) 2970-2980.[8] G.Ramakrishna, T.Sundararajan, “ Impact strength of a few natural fibre reinforced cement mortar slabs: a comparative study”,Cement and Concrete Composites 27 (2005) 547-553.[9] G.R. Williamson, “The effect of steel fibres on compressive strength of the concrete,” Fibre Reinforced Concrete, AmericanConcrete Institude, Detroit, MI, (1974) pp. 195-207 (ACI).[10] H. Krenchel, S.P. Shah, Restrained shrinkage tests with polypropylene fibre reinforced concrete, in: S.P. Shah, G.B. Baston (Eds.),Fibre Reinforced Concrete and Applications, American Concrete Institute SP-105, Detroit, 1987, pp. 141–158[11] Indian Standard Code of practices for plain and reinforced concrete IS: 456:2000.[12] Indian Standard methods of physical test for hydraulic cement. IS: 4031 (Part 6)-1988.[13] Indian Standard methods of test for aggregates for concrete. IS: 2386 (Part-6)-2007.[14] Indian Standard methods of chemical analysis of hydraulic cement. IS: 4032 (1985).[15] Indian Standard recommended guidelines for concrete mix design. IS: 10262-1982.[16] Indian Standard methods of tests for strength of concrete. IS: 516 (1991).[17] LI Bei-xing, Chen Ming-xiang Cheng Fang Liu Lu-ping. “ The mechanical properties of Fibre Reinforced concrete”, Journal ofWuhan University of Technology (May 2004) vol. 19 No.3[18] Lars Kutzign, Gert Konig, “Design Principals of steel fibre reinforced concrete- A Fracture Mechanics Approach”, Leipzig AnnualCivil Engineering Report LACER, vol.3 (1999).[19] Machine Hsiea, Chijen Tua, P.S.Song, “Mechanical properties of polypropylene hybrid fibre-reinforced concrete”, Material Scienceand Engineering A 494 (2008) 153-157.[20] Menon and Pillai, “Reinforced concrete design”, published by Tata McGraw-Hill Company (2007).[21] Nguyen Van Chanh, “Steel fibre reinforced concrete”, Advances in concrete technology volume 3- Gordon and Breach Sciencepublishes.[22] Naaman, A.E and Najm, “bond sleep mechanism of steel fibre in concrete”, ACI material journal (1992), vol. 88 pp. 135-145.[23] T. Budi Aulia, “Effect of polypropylene Fibres on the properties of high strength concretes”, Institutes for Massivbau andBaustoffechnologi, University Leipzig, Lacer No. 7 (2002).[24] T.S.Lok and J.R.Xiao, “Flexural strength assessment of steel fibre reinforced concrete,” Journal of material in civil engineering,vol.11, No.3 (1999).[25] Tantary, M.A.Ramajan, B.Upadhyay A and Prasad, J, “Mechanical properties of steel fibre based concrete”, second nationalconference on recent Advances in Civil Engineering, Kochi, India (2006), pp.27-33.[26] V M Malhortra, Carette, A Bilodeaue, “Mechanical properties and durability of Polypropylene fibre reinforced high-volume fly ashconcrete for shotcrete applications”, ACI Materials Journal,1994,91(5) 478-486.[27] Waheeb Ahmed Al-Khaja. “Mechanical properties and time dependant deformation of polypropylene fibre concrete.” J.King Univ,Vol. 7 Eng Sci. (1) pp 67-76.[28] Yeol Choia, Robert L. Yuan, “Experimental relationship between splitting tensile strength and compressive strength of GFRC andPFRC”, Cement and Concrete Research 35 (2005) 1587-1591.[29] Youjiang Wang, “modeling of fibre pull-out from a cement matrix”, International journal of cement composites and light weightconcrete, Volume 10 No.3.

No public clipboards found for this slide

×
### Save the most important slides with Clipping

Clipping is a handy way to collect and organize the most important slides from a presentation. You can keep your great finds in clipboards organized around topics.

Be the first to comment